SlideShare verwendet Cookies, um die Funktionalität und Leistungsfähigkeit der Webseite zu verbessern und Ihnen relevante Werbung bereitzustellen. Wenn Sie diese Webseite weiter besuchen, erklären Sie sich mit der Verwendung von Cookies auf dieser Seite einverstanden. Lesen Sie bitte unsere Nutzervereinbarung und die Datenschutzrichtlinie.

SlideShare verwendet Cookies, um die Funktionalität und Leistungsfähigkeit der Webseite zu verbessern und Ihnen relevante Werbung bereitzustellen. Wenn Sie diese Webseite weiter besuchen, erklären Sie sich mit der Verwendung von Cookies auf dieser Seite einverstanden. Lesen Sie bitte unsere unsere Datenschutzrichtlinie und die Nutzervereinbarung.

Diese Präsentation wurde erfolgreich gemeldet.

Diese Präsentation gefällt Ihnen? Dann am besten gleich teilen!

rolling of metals

Keine Downloads

Aufrufe insgesamt

19.028

Auf SlideShare

0

Aus Einbettungen

0

Anzahl an Einbettungen

7

Geteilt

0

Downloads

1.007

Kommentare

0

Gefällt mir

71

Keine Notizen für die Folie

- 1. RRoolllliinngg ooff mmeettaallss Chapter 3 • Introduction/objectives • Rolling mills • Classification of rolling processes • Hot rolling • Cold rolling • Forces and geometry relationships in rolling • Simplified analysis of rolling load: Rolling variables • Problems and defects in rolled products • Rolling-mill control • Theories of cold rolling • Theories of hot rolling • Torque and power Subjects of interest Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 2. OObbjjeeccttiivveess • This chapter provides information on different types of metal rolling processes which can also be divided in to hot and cold rolling process. • Mathematical approaches are introduced for the understanding of load calculation in rolling processes. • Finally identification of defects occurring during and its solutions are included. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 3. IInnttrroodduuccttiioonn-- DDeeffiinniittiioonn ooff rroolllliinngg pprroocceessss • Definition of Rolling : The process of plastically deforming metal by passing it between rolls. • Rolling is the most widely used forming process, which provides high production and close control of final product. • The metal is subjected to high compressive stresses as a result of the friction between the rolls and the www.world-aluminium.org Rolling process metal surface. Note: rolling processes can be mainly divided into 1) hot rolling and 2) cold rolling. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 4. IInnttrroodduuccttiioonn-- HHoott aanndd ccoolldd rroolllliinngg pprroocceesssseess Hot rolling • The initial breakdown of ingots into blooms and billets is generally done by hot-rolling. This is followed by further hot-rolling into plate, sheet, rod, bar, pipe, rail. Cold rolling • The cold-rolling of metals has played a major role in industry by providing sheet, strip, foil with good surface finishes and increased mechanical strength with close control of product dimensions. www.vatech.at Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 5. Rolled strips Rollforming machine Sheet rolling machines Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 6. Terminology • Bloom is the product of first breakdown of ingot (cross sectional area > 230 cm2). • Billet is the product obtained from a further reduction by hot rolling (cross sectional area > 40x40 mm2). • Slab is the hot rolled ingot (cross sectional area > 100 cm2 and with a width ≥ 2 x thickness). Suranaree University of Technology Jan-Mar 2007 Semi-finished products • Plate is the product with a thickness > 6 mm. • Sheet is the product with a thickness < 6 mm and width > 600 mm. • Strip is the product with a thickness < 6 mm and width < 600 mm. Further rolling steps Mill products Bloom Billet Slap Plate Sheet Strip Tapany Udomphol
- 7. Mill rolls Mill rolls Rolls Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 8. Ring rolls • Ring rolls are used for tube rolling, ring rolling. • Ring rolls are made of spheroidized graphite bainitic and pearlitic matrix or alloy cast steel base. Cantilever mill roll Tube mill roll Universal roll Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 9. Typical arrangement of rollers for rolling mills Two-high mill, pullover The stock is returned to the entrance for further reduction. Two-high mill, reversing The work can be passed back and forth through the rolls by reversing their direction of rotation. Three-high mill Four-high mill Small-diameter rolls (less strength & rigidity) are supported by larger-diameter backup rolls Cluster mill or Sendzimir mill Consist of upper and lower driven rolls and a middle roll, which rotates by friction. Each of the work rolls is supported by two backing rolls. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 10. Typical arrangement of rollers for rolling mills Continuous rolling • Use a series of rolling mill and each set is called a stand. • The strip will be moving at different velocities at each stage in the mill. σb A four stand continuous mill or tandem mil. σf • The speed of each set of rolls is synchronised so that the input speed of each stand is equal to the output speed of preceding stand. • The uncoiler and windup reel not only feed the stock into the rolls and coiling up the final product but also provide back tension and front tension to the strip. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 11. Typical arrangement of rollers for rolling mills Planetary mill • Consist of a pair of heavy backing rolls surrounded by a large number of planetary rolls. • Each planetary roll gives an almost constant reduction to the slab as it sweeps out a circular path between the backing rolls and the slab. • As each pair of planetary rolls ceases to have contact with the work piece, another pair of rolls makes contact and repeat that reduction. • The overall reduction is the summation of a series of small reductions by each pair of rolls. Therefore, the planetary mill can hot reduces a slab directly to strip in one pass through the mill. • The operation requires feed rolls to introduce the slab into the mill, and a pair of planishing rolls on the exit to improve the surface finish. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 12. RRoolllliinngg mmiillllss Rolling mill is a machine or a factory for shaping metal by passing it through rollers A rolling mill basically consists of • rolls • bearings • a housing for containing these parts • a drive (motor) for applying power to the rolls and controlling the speed • Requires very rigid construction, large motors to supply enough power (MN). Successive stands of a large continuous mill Modern rolling mill + Huge capital investment • skills • engineering design • construction Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 13. Different types of rolling processes There are different types of rolling processes as listed below; • Continuous rolling • Transverse rolling • Shaped rolling or section rolling • Ring rolling • Powder rolling • Continuous casting and hot rolling • Thread rolling Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 14. Conventional hot or cold-rolling The objective is to decrease the thickness of the metal with an increase in length and with little increase in width. • The material in the centre of the sheet is constrained in the z direction (across the width of the sheet) and the constraints of undeformed shoulders of material on each side of the rolls prevent extension of the sheet in the width direction. • This condition is known as plane strain. The material therefore gets longer and not wider. • Otherwise we would need the width of a football pitch to roll down a steel ingot to make tin plate! σy σz σx Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 15. Transverse rolling • Using circular wedge rolls. • Heated bar is cropped to length and fed in transversely between rolls. • Rolls are revolved in one direction. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 16. Shaped rolling or section rolling • A special type of cold rolling in which flat slap is progressively bent into complex shapes by passing it through a series of driven rolls. • No appreciable change in the thickness of the metal during this process. • Suitable for producing moulded sections such as irregular shaped channels and trim. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 17. Shaped rolling or section rolling A variety of sections can be produced by roll forming process using a series of forming rollers in a continuous method to roll the metal sheet to a specific shape Applications: - construction materials, - partition beam - ceiling panel - roofing panels. - steel pipe - automotive parts - household appliances - metal furniture, - door and window frames - other metal products. www.formtak.com A variety of rolled sections Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 18. Ring rolling Seamless rings Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 19. Simulation of ring rolling www.qcforge.com www.rz.rwth-aachen.de Simulation of ring rolling • The donut shape preform is placed between a free turning inside roll and a driven outside roll. • The ring mills make the section thinner while increasing the ring diameter. Relative strain www.shape.co.kr in ring rolling Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 20. Seamless ring rolling Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 21. Powder rolling Metal powder is introduced between the rolls and compacted into a ‘green strip’, which is subsequently sintered and subjected to further hot-working and/or cold working and annealing cycles. Advantage : - Cut down the initial hot-ingot breakdown step (reduced capital investment). - Economical - metal powder is cheaply produced during the extraction process. - Minimise contamination in hot-rolling. - Provide fine grain size with a minimum of preferred orientation. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 22. Continuous casting and hot rolling • Metal is melted, cast and hot rolled continuously through a series of rolling mills within the same process. • Usually for steel sheet production. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 23. Thread rolling • Dies are pressed against the surface of cylindrical blank. As the blank rolls against the in-feeding die faces, the material is displaced to form the roots of the thread, and the displaced material flows radially outward to form the thread's crest. • A blank is fed between two grooved die plates to form the threads. • The thread is formed by the axial flow of material in the work piece. The grain structure of the material is not cut, but is distorted to follow the thread form. • Rolled threads are produced in a single pass at speeds far in excess of those used to cut threads. • The resultant thread is very much stronger than a cut thread. It has a greater resistance to mechanical stress and an increase in fatigue strength. Also the surface is burnished and work hardened. Cut thread and rolled thread Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 24. HHoott--rroolllliinngg • The first hot-working operation for most steel products is done on the primary roughing mill (blooming, slabbing or cogging mills). • These mills are normally two-high reversing mills with 0.6-1.4 m diameter rolls (designated by size). Plate rolling www.msm.cam.ac.uk • The objective is to breakdown the cast ingot into blooms or slabs for subsequent finishing into bars, plate or sheet. • In hot-rolling steel, the slabs are heated initially at 1100 -1300 oC. The temperature in the last finishing stand varies from 700 - 900 oC, but should be above the upper critical temperature to produce uniform equiaxed ferrite grains. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 25. Example for hot strip mill process www.nzsteel.co.nz Oxidation scale is removed Mill reverses after each pass (5 or 7) and the roll gap is reduced each time Slabs are organised according to rolling schedule Red hot slab 210 mm thick is ready for rolling Slab is reduced to a long strip approx 25 mm thick The strip is coiled and uncoiled to make the tail end lead Leading edge and tail The strip is progressively reduced end are removed to the required thicknesses Strip is coiled and up ended or passed through if heavy plate Plate 12 to 30 mm thick Coiled steel 1.8 to 12 mm thk 910 mm to 1550 mm wide Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 26. • Flat plate of large thickness (10-50 mm) is passed through different set of working rolls, while each set consecutively reduces thickness. www.uksteel.org.uk Hot rolled coil produced on strip mill www.reverecopper.com Plate rolling • Hot strip is coiled to reduce its increasing length due to a reduction of thickness. • Reducing the complication of controlling strips of different speeds due to different thicknesses. (thinner section moves faster) Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 27. CCoolldd--rroolllliinngg • Cold rolling is carried out under recrystallisation temperature and introduces work hardening. • The starting material for cold-rolled steel sheet is pickled hot-rolled breakdown coil from the continuous hot-strip mill. www.williamsonir.com • The total reduction achieved by cold-rolling generally will vary from about 50 to 90%. • The reduction in each stand should be distributed uniformly without falling much below the maximum reduction for each pass. • Generally the lowest percentage reduction is taken place in the last pass to permit better control of flatness, gage, and surface finish. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 28. Example for cold strip mill process. www.nzsteel.co.nz In batches of 9 coils, cold rolled steel is annealed to reduce work hardening The 6 roll configuration enables this high speed mill to produce steel of high quality with consistent shape and flatness Cold rolling mill Coils are transferred to and from the annealing furnace The combination mill has a dual function, cold rolling and single pass temper rolling Temper rolling improves the shape of the strip after its workability has been improved by annealing Cold rolled, annealed and tempered coils are transferred to the Cold Finishing Section Cold rolling reduces the thickness and increases the strength of hot rolled steel. The surface finish and shape improve and work hardening results Coils up to 40 tones enter on a conveyor from the pickle line 20 tonne coils of cold rolled steel are dispatched to Metal Coating Line Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 29. CCoolldd--rroolllliinngg • Cold rolling provide products with superior surface finish (due to low temperature no oxide scales) • Better dimensional tolerances compared with hot-rolled products due to less thermal expansion. • Cold-rolled nonferrous sheet may be produced from hot-rolled strip, or in the case of certain copper alloys it is cold-rolled directly from the cast state. Cold rolled strips Cold rolled metals are rated as ‘temper’ • Skin rolled : Metal undergoes the least rolling ~ 0.5-1% harden, still more workable. • Quarter hard : Higher amount of deformation. Can be bent normal to rolling direction without fracturing • Half hard : Can be bent up to 90o. • Full hard : Metal is compressed by 50% with no cracking. Can be bent up to 45o. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 30. Fundamental concept of metal rolling 1) The arc of contact between the rolls and the metal is a part of a circle. 2) The coefficient of friction, μ, is constant in theory, but in reality μ varies along the arc of contact. 3) The metal is considered to deform plastically during rolling. 4) The volume of metal is constant before and after rolling. In practical the volume might decrease a little bit due to close-up of pores. 5) The velocity of the rolls is assumed to be constant. 6) The metal only extends in the rolling direction and no extension in the width of the material. 7) The cross sectional area normal to the rolling direction is not distorted. Assumptions o R α y vo x vf hf ho Lp o x y Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 31. Forces and geometrical rreellaattiioonnsshhiippss iinn rroolllliinngg o R α x y vo vf hf ho Lp o x y • A metal sheet with a thickness ho enters the rolls at the entrance plane xx with a velocity vo. • It passes through the roll gap and leaves the exit plane yy with a reduced thickness hf and at a velocity vf. • Given that there is no increase in width, the vertical compression of the metal is translated into an elongation in the rolling direction. • Since there is no change in metal volume at a given point per unit time o o f f throughout the process, therefore bh v = bhv = bh v …Eq.1 Where b is the width of the sheet v is the velocity at any thickness h intermediate between ho and hf. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 32. vo R x y vf hf ho x’ y’ From Eq.1 o o f f bh v = bh v Given that bo = bf L o f h = h t L t f o Then we have o o f f v h = v h v f = …Eq.2 h h o o f v vo vf When ho hf , we then have vo vf The velocity of the sheet must steadily increase from entrance to exit such that a vertical element in the sheet remain undistorted. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 33. • At only one point along the surface of contact between the roll and the sheet, two forces act on the metal: 1) a radial force Pr and 2) a tangential frictional force F. • If the surface velocity of the roll vr equal to the velocity of the sheet, this point is called neutral point or no-slip point. For example, point N. • Between the entrance plane (xx) and the neutral point the sheet is moving slower than the roll surface, and the tangential frictional force, F, act in the direction (see Fig) to draw the metal into the roll. • On the exit side (yy) of the neutral point, the sheet moves faster than the roll surface. The direction of the frictional fore is then reversed and oppose the delivery of the sheet from the rolls. x Pr N point : vroll = vsheet F α θ β Friction acts in y N x y opposite directions Tapany Udomphol Suranaree University of Technology Jan-Mar 2007
- 34. Pr is the radial force, with a vertical component P (rolling load - the load with which the rolls press against the metal). The specific roll pressure, p, is the rolling load divided by the contact area. P p = …Eq.3 p bL Where b is the width of the sheet. Lp is the projected length of the arc of contact. ( ) ( ) [ ( )] − = − − 1 2 L R h R h h h h L R h h p o f o f p o f ≈
- 35. ≈ − 1 2 2 4 …Eq.4 Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 36. • The distribution of roll pressure along the arc of contact shows that the pressure rises to a maximum at the neutral point and then falls off. • The pressure distribution does not come to a sharp peak at the neutral point, which indicates that the neutral point is not really a line on the roll surface but an area. vo N R hf ho p A B Friction hill in rolling • The area under the curve is proportional to the rolling load. • The area in shade represents the force required to overcome frictional forces between the roll and the sheet. • The area under the dashed line AB represents the force required to deform the metal in plane homogeneous compression. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 37. Roll bite condition For the workpiece to enter the throat of the roll, the component of the friction force must be equal to or greater than the horizontal component of the normal force. cosα sinα r F ≥ P α α sin ≥ ≥ α tan cos F r P But we know r F = μP Therefore μ = tanα Prsineα α Pr α Fcosα F α The angle of bite or the angle of contact F is a tangential friction force Pr is radial force …Eq.5 • If tan α μ, the workpiece cannot be drawn. • If μ = 0, rolling cannot occur. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 38. Therefore Free engagement will occur when μ tan α Increase the effective values of μ , for example grooving the rolls parallel to the roll axis. Using big rolls to reduce tan α or if the roll diameter is fixed, reduce the ho + α1 α1αααα α2 2 Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 39. From triangle ABC, we have = + − 2 2 2 R L R a ( ) p = − − + 2 2 2 2 L R R Ra a ( 2 ) p = − 2 2 L 2 Ra a p As a is much smaller than R, we can then ignore a2. L Ra R h p ≈ 2 ≈
- 40. Where
- 41. h = ho – hf = 2a …Eq.6 A α a h R R-a B C Lp v D o Lp
- 42. h 2 μ tanα ( h) R …Eq.7
- 43. R h Suranaree University of Technology Jan-Mar 2007 ho The critical variables are Lp and h A large diameter roll will permit a thicker slab to enter the rolls than will a small-diameter roll. R R h R h ≈ −
- 44. ≈ −
- 45. = = / 2 / 2 max
- 46. = μ The maximum reduction Tapany Udomphol
- 47. Problem with roll flattening When high forces generated in rolling are transmitted to the workpiece through the rolls, there are two major types of elastic distortions: 1) The rolls tends to bend along their length because the workpiece tends to separate them while they are restrained at their ends. thickness variation. 2) The rolls flatten in the region where they contact the workpiece. The radius of the curvature is increased R R’. (roll flattening) According to analysis by Hitchcock, CP − = + ( ) 1 ' ' o f b h h R R Where C = 16(1-ν2)/πE = 2.16 x 10-11 Pa-1 for steel rolls. Rollling R R ‘ P’ = rolling load based on the deformed roll radius. Roll flattening Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 48. Example: Determine the maximum possible reduction for cold-rolling a 300 mm-thick slab when μ = 0.08 and the roll diameter is 600 mm. What is the maximum reduction on the same mill for hot rolling when μ = 0.5? From Eq.7, ( h) R 2 max
- 49. = μ ( h) (0.08) (300) 1.92mm 2 max For cold-rolling
- 50. = = For hot-rolling ( h) (0.5) (300) 75mm 2 max
- 51. = = Alternatively, we can use the relationship below ( ) Lp α = = α = − μ
- 52. 1 sin , tan R
- 53. h = mm R h R 1.92 Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 54. Simplified analysis ooff rroolllliinngg llooaadd The main variables in rolling are: • The roll diameter. • The deformation resistance of the metal as influenced by metallurgy, temperature and strain rate. • The friction between the rolls and the workpiece. • The presence of the front tension and/or back tension in the plane of the sheet. We consider in three conditions: 1) No friction condition 2) Normal friction condition 3) Sticky friction condition Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 55. 1) No friction situation In the case of no friction situation, the rolling load (P) is given by the roll pressure (p) times the area of contact between the metal and the rolls (bLp). P pbL b R h p o = =σ '
- 56. Where the roll pressure (p) is the yield stress in plane strain when there is no change in the width (b) of the sheet. …Eq.8 Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 57. 2) Normal friction situation In the normal case of friction situation in plane strain, the average pressure p can be calculated as. _ = Q − ( 1) 1 _ ' o e Q p σ …Eq.9 Where Q = μLp/h h = the mean thickness between entry and exit from the rolls. From Eq.8, _ = p P pbL ( ) 1 2 _σ We have …Eq.10 = e − b R
- 58. h P Q o 1 Q 3 Roll diameter Rolling load Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 59. •Therefore the rolling load P increases with the roll radius R1/2, depending on the contribution from the friction hill. • The rolling load also increases as the sheet entering the rolls becomes thinner (due to the term eQ). • At one point, no further reduction in thickness can be achieved if the deformation resistance of the sheet is greater than the roll pressure. The rolls in contact with the sheet are both severely elastically deformed. • Small-diameter rolls which are properly stiffened against deflection by backup rolls can produce a greater reduction before roll flattening become significant and no further reduction of the sheet is possible. Backup rolls Example: the rolling of aluminium cooking foil. Roll diameter 10 mm with as many as 18 backing rolls. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 60. • Frictional force is needed to pull the metal into the rolls and responsible for a large portion of the rolling load. • High friction results in high rolling load, a steep friction hill and great tendency for edge cracking. • The friction varies from point to point along the contact arc of the roll. However it is very difficult to measure this variation in μ, all theory of rolling are forced to assume a constant coefficient of friction. • For cold-rolling with lubricants, μ ~ 0.05 – 0.10. • For hot-rolling , μ ~ 0.2 up to sticky condition. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 61. Example: Calculate the rolling load if steel sheet is hot rolled 30% from a 40 mm-thick slab using a 900 mm-diameter roll. The slab is 760 mm wide. Assume μ = 0.30. The plane-strain flow stress is 140 MPa at entrance and 200 MPa at the exit from the roll gap due to the increasing velocity. x − − (40) ( h ) h h o f = h mm x = = h h h mm (40) (28) (0.30) 450 12 R h μ L p μ Q _ _ = = 140 200 ' ' ' = =σ −
- 62. P Q e b R h Q o 1 = − Suranaree University of Technology Jan-Mar 2007 h o f f f o (40) (28) 12 28 100 30 (40) 100 30%
- 63. = − = − = mm h h h o f 34 2 2 _ = + = + = 0.65 (34)
- 64. = = x h h MPa entrance exit o 170 2 2 + = + = σ σ σ P (e 1 ) (0.76) 0.45 x 0.012 13.4 MN (0.65) 170 ( 1) 1 0.65 ' = From Eq.10 Tapany Udomphol
- 65. 3) Sticky friction situation What would be the rolling load if sticky friction occurs? Continuing the analogy with compression in plane strain L = + 1 p p + = σ o 1 σ ' 0 a 2 _ _ = h P pbLp From Eq.8, 4 ' _ h From example; =σ ' P o P
- 66. R h _ h 1 4 + 0.45 0.012
- 67. = + 4 0.034 170 = P MN 1 (0.76) 0.45 x 0.012 x x b R h 14.6 Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 68. Example: The previous example neglected the influence of roll flattening under very high rolling loads. If the deformed radius R’ of a roll under load is given in Eq.11, using C = 2.16x10-11 Pa-1, P’ =13.4 MPa from previous example. CP ' ' 1 …Eq.11 ( ) − = + o f b h h R R Where C = 16(1-ν2)/πE ,P’ = Rolling load based on the deformed roll radius. ( ) m − 11 6 2.16 x 10 13.4 x 10 ' = + = R 0.464 0.76 x 0.012 0.45 1 We now use R’ to calculate a new value of P’ and in turn another value of R’ 0.30 464 12 = = 34 ( ) x
- 69. R h _ h Q = μ 1 = − 0.66 '' 0.66 = P e x MN 1 0.76 0.464 0.012 13.7 m − 11 6 x x 0.66 2.16 10 (13.7 10 ) x R 0.465 0.76 0.012 170 = + 0.45 1 '' = The difference between the two estimations of R’ is not large, so we stop the calculation at this point. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 70. Relationship of μ, rolling load and torque • We have known that the location of the neutral point N is where the direction of the friction force changes. • If back tension is applied gradually to the sheet, the neutral point N shifts toward the exit plane. • The total rolling load P and torque MT (per unit of width b) is given by x N point : vroll = vsheet Pr F N α β θ y Friction acts in opposite directions Lp x y pdx p p ( ) L p ∫ ∫ ∫ 0 = = = M L o T PR P b M = T b thus P b L μ μ μ pdx R R pdx R o = μ Where μ is obtained by measuring the torque and the rolling load at constant roll speed and reduction with the proper back tension. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 71. Back and front tteennssiioonnss iinn sshheeeett • The presence of back and front tensions in the plane of the sheet reduces the rolling load. • Back tension may be produced by controlling the speed of the uncoiler relative to the roll speed. Back tension, σb Front tension, σf Uncoiler Coiler p σ’ o σ’ o σ’ o- σb σ’ o- σf • Front tension may be created by controlling the coiler. • Back tension is ~ twice as effective in reducing the rolling load P as front tension. • The effect of sheet tension on reducing rolling pressure p can be shown simply by _ 2 p =σ ' o −σ h = σ o −σ h 3 …Eq.11 • If a high enough back tension is applied, the neutral point moves toward the roll exit – rolls are moving faster than the metal. • If the front tension is used, the neutral point will move toward the roll entrance. Where σh = horizontal sheet tension. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 72. Problems and ddeeffeeccttss iinn rroolllleedd pprroodduuccttss Defects from cast ingot before rolling Defects other than cracks can result from defects introduced during the ingot stage of production. • Porosity, cavity, blow hole occurred in the cast ingot will be closed up during the rolling process. • Longitudinal stringers of non-metallic inclusions or pearlite banding are related to melting and solidification practices. In severe cases, these defects can lead to laminations which drastically reduce the strength in the thickness direction. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 73. Defects during rolling There are two aspects to the problem of the shape of a sheet. 1) Uniform thickness over the width and thickness – can be precisely controlled with modern gage control system. h h 2) Flatness – difficult to measure accurately. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 74. Uniform thickness • Under high rolling forces, the rolls flatten and bend, and the entire mill is elastically distorted. • Mill spring causes the thickness of the sheet exiting from the rolling mill to be greater than the roll gap set under no-load conditions. • Precise thickness rolling requires the elastic constant of the mill. Calibration curves are needed, see Fig. (1–3 GNm-1 for screw-loaded rolling mills, 4 GNm-1 for hydraulically loaded mills). Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 75. • Roll flattening increases the roll pressure and eventually causes the rolls to deform more easily than the metal. •The limiting thickness is nearly proportional to μ, R, σ’ o but inversely proportional to E. For example in steel rolls the limiting thickness is given by _ ' μ R σ o = …Eq.12 12.8 min h In general, problems with limiting gauge can be expected when the sheet thickness is below 1/400 to 1/600 of the roll diameter. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 76. Flatness • The roll gap must be perfectly parallel to produce sheets/plates with equal thickness at both ends. • The rolling speed is very sensitive to flatness. A difference in elongation of one part in 10,000 between different locations in the sheet can cause waviness. Rolling direction Perfectly flat More elongated along edges More elongated in the centre Suranaree University of Technology Jan-Mar 2007 Tapany Udomphol
- 77. Solutions to flatness problems • Camber and crown can be used to correct the roll deflection (at only one value of the roll force). Or use rolling mill equipped with hydraulic jacks to permit the elastic distortion of the rolls to correct deflection. (a) (b) (a) The use of cambered rolls to compensate for roll bending. (b) Uncambered rolls give variation of thickness. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 78. • Hot mill can be provided with facilities for crown control to improve the control of the profile of hot strip mill. • For example work roll bending with continuous variable crown and pair cross mills. •The roll cross angle of rolls incorporated in a stand of each rolling mill is set at a predetermined value beforehand. • If there is a roll cross angle that will enable a target sheet crown to be applied to each sheet and the roll bender load of each stand is adjusted on-line, thereby effecting sheet crown control. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 79. Possible effects when rolling with insufficient camber (a) (b) (c) (d) (e) • Thicker centre means the edges would be plastically elongated more than the centre, normally called long edges. • This induces the residual stress pattern of compression at the edges and tension along the centreline. • This can cause centreline cracking (c), warping (d) or edge wrinkling or crepe-paper effect or wavy edge (e). Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 80. Possible effects when rolls are over-cambered. (a) (b) (c) (d) (e) • Thicker edges than the centre means the centre would be plastically elongated more than the edges, resulting in lateral spread. •The residual stress pattern is now under compression in the centreline and tension at the edges (b). • This may cause edge cracking (c), centre splitting (d), centreline wrinkling (e). Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 81. • Shape problems are greatest when rolling in thin strip (0.01 in) because fractional errors in the roll gap profile increase with decrease in thickness, producing larger internal stress. • Thin sheet is also less resistant to buckling. • Mild shape problems may be corrected by stretch levelling the sheet in tension or by bend flexing the sheet in a roller-leveller, see Fig. two high Material flow adjustable work rolls Roller-leveller Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 82. • Edging can also be caused by inhomogeneous deformation in the thickness direction. • If only the surface of the workpiece is deformed (as in a light reduction on a thick slab), the edges are concaved (a). The overhanging material is not compressed in the subsequent step of rolling, causing this area under tensile stress and leading to edge cracking. This has been observed in initial breakdown of hot-rolling when h/Lp 2 • With heavy reduction, the centre tends to expand more laterally than the surface to produced barrelled edges (b). This causes secondary tensile stresses by barrelling, which are susceptible to edge cracking. • Alligatoring (c) will occur when lateral spread is greater in the centre than the surface (surface in tension, centre in compression) and with the presence of metallurgical weakness along the centreline. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 83. • Surface defects are more easily in rolling due to high surface to volume ratio. Grinding , chipping or descaling of defects on the surface of cast ingots or billets are recommended before being rolled. • Laps due to misplace of rolls can cause undesired shapes. Roll misplacement • Flakes or cooling cracks along edges result in decreased ductility in hot rolling such as blooming of extra coarse grained ingot. • Scratches due to tooling and handling. • Variation in thickness due to deflection of rolls or rolling speed. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 84. RRoolllliinngg mmiillll ccoonnttrrooll • Modern continuous hot-strip and cold rolling mills operated under automatic control provide high throughput and production rate. • Of all the metal working processes, rolling is the best suited for the adoption of automatic control because it is an essentially steady-state process in which the tooling geometry (roll gap) may be changed readily during the process. • Automatic control in rolling such as the development of online sensors to continuously measure sheet thickness. The most widely used instruments are 1) flying micrometer 2) x-ray or isotope, gauges which measure thickness by monitoring the amount of radiation transmitted through the sheet. • More recently control procedures have been aimed at controlling strip shape as well as thickness. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 85. Problem of gauge control Plastic curve Elastic curve 1 2 _σ = e − b R
- 86. h P Q o 1 Suranaree University of Technology Jan-Mar 2007 P Roll gap Sheet thickness Rolling load hf ho Characteristic elastic and plastic curves for a rolling mill • For a given set of rolling conditions, the rolling load varies with the final sheet thickness, according to the plastic curve, which can be obtained in Eq.10. ( ) Q 3 • The elastic curve for mill spring indicates that a sheet of initial thickness ho will have a final thickness hf and the load on the mill would be P in normal situation. Normal situation Tapany Udomphol
- 87. Situation where μ or flow stress increase Elastic curve Use of characteristic curves to show changes in rolling condition. μ due to lubricant breakdown σ due to Temp The plastic curve will be raised. Therefore rolling load P1 P2 final thickness hf1 hf2 In order to maintain a constant thickness hf1, under these new condition, the roll gap would have to be decreased. This moves the elastic curve to the left and further increases the rolling load to P3. • If the sheet thickness increases, the plastic curve will move to the right relative to the elastic curve. • If the there is an increase in strip tension, the plastic curve will move to the left. Example: Suranaree University of Technology Jan-Mar 2007 P1 Sheet thickness Rolling load hf1 ho P2 hf2 New roll gap P3 Increase in μ or σ Tapany Udomphol
- 88. Thickness measurement in continuous hot mill • In a continuous hot mill, the strip thickness is measured indirectly by measuring the rolling load and using the characteristic curve of the mill to establish the thickness. • The error signal is fedback to the rolling mill screws to reposition them so as to minimise the error. • An x-ray gauge is used after the last stand to provide an absolute measurement of sheet gauge. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 89. Thickness measurement in continuous cold strip mills • Thickness is measured by x-ray gauges while the error in the thickness following the first stand is usually fedback to adjust the gap sitting on the first stand. • Gauge control in subsequent stands usually is achieved by controlling the strip tension through controlling the relative roll speed in successive stands or the coiler speed. • Gauge control through control of strip tension has faster response time than control through change in roll setting. sensors Thickness gauging is achieved by using two opposing sensors with laser spots aimed at opposite sides of a target. The sensor readings are subtracted from the sensor separation distance to yield a real-time thickness measurement. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 90. Theory ooff ccoolldd rroolllliinngg A theory of rolling is aimed at expressing the external forces, such as the rolling load and the rolling torque, in terms of the geometry of the deformation and the strength properties of the material being rolled. Assumptions 1) The arc of the contact is circular – no elastic deformation of the roll. 2) The coefficient of friction is constant at all points on the arc of contact. 3) There is no lateral spread, so that rolling can be considered a problem in plain strain. 4) Plane vertical section remain plane: i.e., the deformation is homogeneous. 5) The peripheral velocity of the rolls is constant 6) The elastic deformation of the sheet is negligible in comparison with the plastic deformation. 7) The distortion-energy criterion of yielding, for plane strain, holds. σ −σ = σ ' Yield stress in plane 1 3 o =σ o 2 3 strain condition Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 91. The stresses acting on an element of strip in the roll gap dθ o θ ho h+dh h hf B σx+dσx σx Prcosθ θ Pr μPr μPrsinθ μPrcosθ Prsinθ R dθ • At any point of contact between the strip and the roll surface, designated by the angle θ, the stresses are the radial pressure pr and the tangential shearing stress τ = μpr. These stresses are resolved into their horizontal and vertical components (b). • The stress σx is assumed to be uniformly distributed over the vertical faces of the element. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 92. R dθ Prsinθ θ Prcosθ Pr μPrcosθ σx+dσx σx h+dh h μPr μPrsinθ μPrsinθ θ Prcosθ Pr μPrcosθ Prsinθ R dθ R dθ PrsinθRdθ σxh Unit length μPrcosθRdθ (σx+dσx)(h+dh) Pr μP PrsinθRdθ rcosθRdθ Taking summation of the horizontal forces on the element results in (σ dσ )(h dh) μp θRdθ σ h p θRdθ x x r x r + + + 2 cos = + 2 sin ( σ ) = 2 p R ( sin θ ± μ cos θ ) θ d h d r x Which simplifies to …Eq.14 Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 93. The forces acting in the vertical direction are balanced by the specific roll pressure p. Taking the equilibrium of forces in the vertical direction results in a relationship between the normal pressure and the radial pressure. (1m μ tanθ ) r p = p …Eq.14 The relationship between the normal pressure and the horizontal compressive stress σx is given by the distortion energy criterion of yielding for plane strain. σ 1 −σ 3 = σ =σ ' o o 2 3 p −σ x =σ ' o …Eq.15 Where p is the greater of the two compressive principal stresses. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 94. The solution of problems in cold rolling are complicated. Some simplification to this problem has been provided by Bland and Ford. By restricting the analysis to cold rolling under conditions of low friction and for angles of contact 6o, then we can put sin θ ~ θ and cos θ ~ 1. Thus Eq.14 can be written ( ( x ) ) (θ μ ) θ ( θ μ ) θ d h σ = ' ± 2 p R x = ' p R ± …Eq.16 σ d h d r d r It is also assumed that pr ~ p , so that Eq.15 can be written σx = pr-σ’ o. By substituting into Eq.16 and integrating, relatively simple equations of the radial pressure result. Roll entrance to neutral point: σ σ xb (H H ) ' μ − p 1 = o − 1 h r e h o σ ' 01 …Eq.17 Neutral point to roll exit: σ σ ' p μ xf H = o − ' h 1 …Eq.18 r e f h σ 02 Where 2 1 ' 2 1 ' R R = − θ f f h 2 tan 1 h H and σxb = back tension σxf = front tension Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 95. The rolling load or total force P is the integral of the specific roll pressure over the arc of contact. θ α ∫ = P = ' R b pd θ …Eq.19 o Where b = width of sheet α = contact angle The solution is replaced by the modern digital computer. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 96. TThheeoorryy ooff hhoott--rroolllliinngg In hot working processes, the flow stress for hot-rolling is a function of both temperature and strain rate (speed of rolls) Calculation of rolling load by Sims ' [ ( )] 1 P =σ o b R h o − h f 2Q p …Eq.20 Where Qp is a complex function of the reduction in thickness and the ratio R/hf. Values of Qp may be obtained from
- 97. 1 π 4 h = − h R h π tan − ln − p 4 h h 2 o
- 98. n o f h f f h h Q …Eq.21 Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 99. TToorrqquuee aanndd ppoowweerr Torque is the measure of the force applied to a member to produce rotational motion. Power is applied to a rolling mill by applying a torque to the rolls and by means of strip tension. The power is spent principally in four ways 1) The energy needed to deform the metal. 2) The energy needed to overcome the frictional force. 3) The power lost in the pinions and power-transmission system. 4) Electrical losses in the various motors and generators. Remarks: Losses in the windup reel and uncoiler must also be considered. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 100. R a P MT = Pa h hf o P a R Schematic diagram illustrating roll torque The total rolling load is distributed over the arc of contact in the typical friction-hill pressure distribution. However the total rolling load can be assumed to be concentrated at a point along the act of contact at a distance a from the line of centres of the rolls. The ratio of the moment arm a to the projected length of the act of contact Lp can be given as a λ = = …Eq.22 p
- 101. R h a L Where λ is 0.5 for hot-rolling and 0.45 for cold-rolling. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 102. The torque MT is equal to the total rolling load P multiplied by the effective moment arm a. Since there are two work rolls, the torque is given by R a P MT = Pa M Pa T = 2 …Eq.23 hf ho P a R During one revolution of the top roll the resultant rolling load P moves along the circumference of a circle equal to 2πa. Since there are two work rolls, the work done W is equal to Work = 2(2πa)P …Eq.24 Since power is defined as the rate of doing work, i.e., 1 W = 1 J s-1, the power (in watts) needed to operated a pair of rolls revolving at N Hz (s-1) in deforming metal as it flows through the roll gap is given by W = 4πaPN …Eq.25 Where P is in newtons and a is in metres. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007
- 103. Example: A 300 mm-wide aluminium alloy strip is hot-rolled in thickness from 20 to 15 mm. The rolls are 1 m in diameter and operate at 100 rpm. The uniaxial flow stress for aluminium alloy can be expressed as σ = 140ε0.2 (MPa). Determine the rolling load and the power required for this hot reduction. From Eq.20 [ ( )] o o f p P b R h h 2Q =σ ' − 1 b = 0.3 m, R = 0.5 m, ho = 0.02 m and hf = 0.015 m, we need to know σ’ o and Qp. 0.288 0.25 = 33.3 20 15 = ε ln 1 − 20 15 20 500 = = 15 k ∫ ε ε + σ ε ' 1 140 0.288 2 1 = − = =
- 104. = = a 0.5 R h 0.5 0.5 x 0.005 0.025 m = = N 100 / 60 1.67 s − − − = 6 1 = 1 π Suranaree University of Technology Jan-Mar 2007 = = r R f h ( ) MPa n n k k d o n o n o n o 91 1.2 ( 1) 1 0.2 ' 1 1 1 1 1 = = + = + = = σ ε ε ε ε ε P (91)(0.3)[0.5(0.020 0.015)] (1.5) 2.36MN 3 2 Qp can be found from graph(~1.5) when reduction r and R/hf are known. W 4 ( 0.025 )( 2.36 x 10 )( 1.67 )Js 1.24 MW Tapany Udomphol
- 105. References • Dieter, G.E., Mechanical metallurgy, 1988, SI metric edition, McGraw-Hill, ISBN 0-07-100406-8. • Edwards, L. and Endean, M., Manufacturing with materials, 1990, Butterworth Heinemann, ISBN 0-7506-2754-9. • Beddoes, J. and Bibbly M.J., Principles of metal manufacturing process, 1999, Arnold, ISBN 0-470-35241-8. • Lecture note, 2003. • Firth Rixson leavelets. • Metal forming processes, Prof Manas. • Metal forming lecture, Ass Prof. P. Srichareonchai. Suranaree University of Technology Tapany Udomphol Jan-Mar 2007

Keine öffentlichen Clipboards für diese Folie gefunden

Sie haben diese Folie bereits ins Clipboard „“ geclippt.

Clipboard erstellen

Als Erste(r) kommentieren